PHYSICAL REVIEW B 1 NOVEMBER 1998-IIVOLUME 58, NUMBER 18 Lattice distortions around a Tl 1 impurity in NaI:Tl 1 and CsI:Tl 1 scintillators: An ab initio study involving large active clusters. Andrés Aguado Departamento de Fı´sica Teo´ rica, Facultad de Ciencias, Universidad de Valladolid, 47011 Valladolid, Spain. Andrés Ayuela Laboratory of Physics, Helsinki University of Technology, 02015 Espoo, Finland. JoséM. López and Julio A. Alonso Departamento de Fı´sica Teo´ rica, Facultad de Ciencias, Universidad de Valladolid, 47011 Valladolid, Spain. ~Received 21 April 1998!. Ab initio perturbed ion cluster-in-the-lattice calculations of the impurity centers NaI:Tl1 and CsI:Tl1 are presented. We study several active clusters of increasing complexity and show that the lattice relaxation around the Tl1 impurity implies the concerted movement of several shells of neighbors. The results also reveal the importance of considering a set of ions that can respond to the geometrical displacements of the inner shells by adapting self-consistently their wave functions. Comparison with other calculations involving comparatively small active clusters serves to assert the significance of our conclusions. Contact with experiment is made by calculating absorption energies. These are in excellent agreement with the experimental data for the most realistic active clusters considered.@S0163-1829~98!09741-0# r ic a b tic c ice lla b. to th th. y. rd. es m th st e l- ti m , o. o O. e er h. ions al g f a. at-. d by. o- the. In en ing . In. ons,. a- nd d ect in. we his red,. er I. INTRODUCTION. The interest in luminescent materials has increased in cent years because of their numerous technolog applications.1 Most of these materials involve the doping of pure ionic crystal, that is, substitution of some of the ions other ions with specific absorption-emission characteris ~Tl1, Ce31, etc.!. The presence of impurity ions in ioni crystals induces geometrical distortions in the host latt Those distortions are an important ingredient in the scinti tion process and thus it is important to establish a relia description of them.. A convenient way to calculate the lattice distortions is model the doped crystal by a finite cluster centered on impurity and embedded in a field representing the rest of host lattice. This cluster approach has been used to stud geometrical and optical properties of doped crystals.2–25 The cluster ~active space! can be studied by using standa quantum-mechanical methods. The rest of the crystal~envi- ronment! can be described in several ways. In the simpl and most frequently used approach, the environment is si lated by placing point charges on the lattice sites, but procedure has to be improved in order to obtain a reali description of the lattice distortions around th impurity.5–8,11,14,17,20,22,23Model potentials have been deve oped to represent the effects of the environment on the ac cluster, which include attractive and repulsive quantu mechanical terms aside from the classical Madelung term26. but a problem still remains: the large computational cost conventional molecular orbital~MO! calculations prevents us from performing an exhaustive geometrical relaxation the lattice around the impurity. In the most accurate M calculations,8,20,22,23,25only the positions of the ions in th first shell around the impurity are allowed to relax. Howev geometrical relaxations far beyond the first shell of neig PRB 580163-1829/98/58~18!/11964~6!/$15.00 e- al. y s. . - le. e e. the. t u- is ic. ve -. f. f. , -. bors can be expected. In fact, recent classical simulat of solids,27–35 performed employing phenomenologic potentials,36–41 have shown the importance of considerin appropriate large-scale lattice relaxations in the study o variety of intrinsic and extrinsic defects in ionic crystals.. In this paper we report theoretical calculations of the l tice distortions induced by a Tl1 impurity in two well-known ionic scintillators, namely, NaI:Tl1 and CsI:Tl1. For this purpose we use theab initio perturbed ion~PI! model,42–46. which circumvents the problems mentioned above:~a! The active cluster is embedded in an environment represente the ab initio model potentials of Huzinagaet al.26 ~b! The computational simplicity of the PI model allows for the ge metrical relaxation of several coordination shells around impurity.11,14. The remainder of this paper is organized as follows: Sec. II we describe the different clusters which have be used in order to assert the influence of the embedd scheme and of the size of the active cluster on the results Sec. III we present and discuss the results of the calculati and Sec. IV summarizes the main conclusions.. II. CALCULATIONAL STRATEGY: DESCRIPTION OF THE DIFFERENT ACTIVE CLUSTERS. The ab initio perturbed ion model is a particular applic tion of the theory of electronic separability of Huzinaga a co-workers,47,48 in which the basic building block is reduce to a single ion. The PI model was first developed for perf crystals.42 Its application to the study of impurity centers ionic crystals has been described in Refs. 11 and 14, and refer to those papers for a full account of the method. In t case, an active cluster containing the impurity is conside and the Hartree-Fock-Roothaan~HFR! equations49 of each ion in the active cluster are solved in the field of the oth 11 964 ©1998 The American Physical Society. tra p fo a e te th t. th ec ul o he to. f in t lf. th i. th b. nt. o g. - si te d. e nt. ro er he le l. 3 co. b. in 3 fir c. in ia. r t. e. ter the. in. e an. ve al. d ly. s: 6. on-. nt y al- ch to are. ets:. ns -. ula- led e. e od. d PI. l PI. the the me e- l. - m. lue. PRB 58 11 965LATTICE DISTORTIONS AROUND A Tl1 IMPURITY . . . ions. The Fock operator includes, apart from the usual in atomic terms, an accurate, quantum-mechanical crystal tential and a lattice projection operator which accounts the energy contribution due to the overlap between the w functions of the ions.50 The atomiclike HFR solutions ar used to describe the active cluster ions in an iterative s wise procedure. Also, as we shall see later in more detail, positions of some ions in the active cluster are allowed relax. The wave functions of the lattice ions external to active cluster are taken from a PI calculation for the perf crystal and kept fixed during the embedded-cluster calc tion. Those wave functions are explicitly considered up t distanced from the center of the active cluster such that t quantum contribution from the most distant frozen shell the effective cluster energy is less than 102 6 hartree. In prac- tice, this means 25 shells for NaI:Tl1 and 21 shells for CsI:Tl1. Ions beyondd contribute to the effective energy o the active cluster just through the long-range Madelung teraction; so they are represented by point charges. At end of the calculation, the ionic wave functions are se consistent within the active cluster and consistent with frozen description of the rest of the lattice. The intraatom Coulomb correlation correction, which is neglected at Hartree-Fock level, is computed by using the Coulom Hartree-Fock~CHF! model of Clementi.51,52 An effective en- ergy can be assigned to each ion that collects all the co butions to the total crystal energy involving that ion.42. In this work we have employed several active clusters increasing complexity and with different embeddin schemes. Now we describe each cluster~see Fig. 1!, first for NaI:Tl1, that is, a substitutional Tl1 impurity in a NaI crys- tal with the rocksalt structure.. ~A! ~TlI 6! 52:PC. This active cluster is formed by the im. purity cation Tl1 and its 6 nearest neighbors, whose po tions are allowed to relax. The rest of the crystal is simula by using point charges~PC’s!. Notice that in this case, an also in cluster (A* ) below, the environment is simplified with respect to the statements at the beginning of this s tion, in the sense that the ‘‘frozen ions’’ are just poi charges.. ~B! ~TlI 6! 52:NaI. The active cluster is the same as in~A!,. but now the environment is represented by ions whose ‘‘f zen’’ wave functions are obtained from a PI calculation p formed for the pure NaI crystal. In the perfect crystal all t cations ~or anions! are equivalent, and there is a sing nearest-neighbor Na-I distance. These characteristics are around the substitutional impurity.. ~C! ~TlI 14Na18! 51:NaI. The active cluster is formed by 3. ions corresponding to the central impurity cation plus 4 ordination shells. The rest of the crystal is represented frozen ions with PI wave functions as in~B!. In the calcula- tions performed on this cluster only the positions of ions the first shell around Tl1 are allowed to relax. The other shells in the cluster provide an interface between the shell and the frozen environment. The ions in this interfa respond to the distortion induced by the impurity by adapt self-consistently their wave functions to the new potent but not their positions.. ~D! ~TlI 92Na86! 52:NaI. This is the largest active cluste. used for this material. It has 179 ions which correspond the central Tl1 cation plus 12 coordination shells. Only th - o- r. ve. p- e. o e t. a- a. - he - e c e -. ri-. f. - d. c-. - -. ost. - y. st e g l,. o. 33 ions of the 4 inner shells relax their positions; the 8 ou shells provide the interface between the inner ones and environment of frozen PI ions.. Next, for CsI:Tl1, that is, a substitutional Tl1 impurity in a CsI crystal with the CsCl structure, we define 4 clusters a similar way.. (A* ) ~TlI 8! 72:PC. The active cluster is formed by th. impurity plus its 8 nearest neighbors, and is embedded in environment of point charges.. (B* ) ~TlI 8! 72:CsI. This cluster is similar to (A* ), but. the environment is now simulated by frozen ions with wa functions taken from a PI calculation for the pure CsI cryst. (C* ) ~TlI 32Cs32! 1:CsI. The active cluster has 65 ions an. is formed by the impurity plus 6 coordination shells. On the positions of the ions in the first shell around Tl1 are allowed to relax. The environment is the same as in (B* ).. (D* ) ~TlI 88Cs92! 41:CsI. The active cluster has 181 ion. the impurity plus 12 coordination shells. The ions in the innermost shells can relax their positions, and the envir ment is as in (B* ).. The geometrical relaxations of the shells in the differe cluster models described above have been performed b lowing for independent breathing displacements for ea shell of ions, and minimizing the total energy with respect those displacements until the effective cluster energies converged up to 1 meV. A downhill simplex algorithm53 was used. For the ions we have used large STO basis s (5s4p) for Na1,54 (11s9p5d) for I2,54 (11s9p5d) for Cs1,55 and (13s9p7d3 f ) for Tl1.55. III. RESULTS AND DISCUSSION. Before presenting the results for the lattice distortio around the Tl1 impurity we test the consistency of the em bedding method for the case of pure~undoped! crystals. For this purpose we compare the results of two sets of calc tions for NaI. In the first one we study the clusters labe ~A!, ~B!, ~C!, and~D! in Sec. II, with the embedding schem indicated there for each case, but with a Na1 cation instead of the Tl1 impurity. This is, of course, just the case of th pure NaI crystal treated by the embedded-cluster meth One can then compare the results with those of a standar calculation for the perfect crystal.42 We can anticipate some differences between the two methods since in the usua calculation for a perfect crystal all the cations~or anions! are equivalent, while in the embedded-cluster description of same system the cation acting as a fictitious impurity and other cations of the crystal are not described in the sa way. This systematic error is, in fact, what we want to r move in the analysis of the distortions around the true, T1, impurities. If we callR1 the distance between the Na. 1 cation and its first I2 neighbors, Table I givesR1 for the four cluster models~A!, ~B!, ~C!, and ~D!, together with the difference DR15@ R1(cluster)2 R1. PI(crystal)# between the embedded cluster result and that of the perfect crystal at equilibriu and the relative deviationDR1 /R1. PI(crystal). The PI model predicts for the crystal an equilibrium valueR1. PI(crystal) of 3.237 Å, in very good agreement with the experimental va R1. expt53.240 Å. The first two cluster schemes,~A! and ~B!, give large distortionsDR1 . In contrast, a contraction ofR1 smaller than 1% occurs for cluster models~C! and ~D!. The. l as. 11 966 PRB 58AGUADO, AYUELA, LÓ PEZ, AND ALONSO FIG. 1. The different active clusters studied; small spheres represent cations and large spheres represent anions:~a! (TlI 6) 52, ~b!. (TlI 14Na18) 51, ~c! (TlI 92Na86). 52, ~d! (TlI 8) 72, ~e! (TlI 32Cs32). 1, and~f! (TlI 88Cs92) 41. These clusters are embedded in the crysta. indicated in the text. i. a io th. ty nd ter ter- conclusions for CsI are similar. A good self-embedding only achieved for clusters~C! and ~D! @(C* ) and (D* )#. Comparison of~B! and ~C! shows the importance of smooth interface between the inner cluster core, where are allowed to move, and the frozen environment around s. ns e. cluster. Comparison of~C! and ~D! establishes the necessi of allowing for relaxation of the radii of several shells arou the impurity. The systematic error that the embedding-clus scheme makes has to be taken into account in order to in pret properly the distortions induced by the Tl1 impurity.. in e. - ns t. d n. n. e i-. a th. k of. h late. rth a. s is. the d our ond. n. -. ell,. ta e. PRB 58 11 967LATTICE DISTORTIONS AROUND A Tl1 IMPURITY . . . Now we present the results for the lattice distortions duced by the Tl1 impurity in NaI and CsI. In this case w have calculated. DRi 5 Ri ~ NaI:Tl 1!2 Ri ~ NaI:Na. 1!, ~1!. where Ri (i 5 1,2,3,. . . ) refer to the radii of the first, sec ond, . . . shells around the impurity and both calculatio have been performed in the embedded-cluster scheme. In way the systematic errors of the cluster method analyze Table I tend to cancel. As before,R1 is the distance betwee the central cluster cation, Tl1 or Na1, and the I2 anions in its first-neighbor shell. For the reasons given above we o trust the results from clusters~C!, ~D! @or (C* ), (D* )# and the results forR1 and DR1 are given in Table II, which also contains results for Tl1 in CsI. Although we discourage th use of models~A! and~B!, just for the purposes of compar son with Berrondoet al.24 we have also calculatedDR1 for NaI:Tl1 in model ~A! and for CsI:Tl1 in model (A* ). Ber- rondo et al. used a similar embedded-cluster scheme, though their calculational method was different, based on. TABLE I. Self-embedding test. Values ofR1 , the radius of the first coordination shell around Na1 in NaI obtained from embedded-cluster calculations, and their deviationsDR1 from the theoretical value obtained in a PI calculation for the perfect crys Relative deviationsDR1 /R1. PI(crystal) are given in brackets. Not the good self-embedding achieved in cluster models~C! and ~D!.. NaI:Na1 Cluster R1 ~Å! DR1 ~Å!. ~A! 3.540 1 0.303 ( 1 9.36%). ~B! 3.159 2 0.078 ( 2 2.41%). ~C! 3.213 2 0.024 ( 2 0.74%). ~D! 3.234 2 0.003 ( 2 0.09%) -. his in. ly. l- e. linear combination of atomic orbitals~LCAO!. Taking as a reference the experimental nearest-neighbor Na1-I2 distance in the bulk, Berrondoet al. obtainedDR15 0.54 Å, and tak- ing the same reference we obtainDR15 0.50 Å. The good agreement between the two calculations provides a chec our theoretical method. However, this large value ofDR1 is partly due to the fact that the calculatedR1(NaI:Tl. 1) and the referenceR1. expt(pure crystal) are not fully consistent wit each other for the reasons discussed above. If we calcu R1(pure NaI) also by using model~A! ~with Na. 1 instead of Tl1!, that is, as in Eq.~1!, then a corrected ‘‘smaller’’ value DR15 0.20 Å ~or 5.6%! results.. Returning to models~C! and~D! we predict, using Eq.~1! a lower expansion ofR1 . In fact, DR1 is equal to 0.039 Å ~1.2% expansion! for model ~D!. However, the distortions are not restricted to the first shell. The second and fou shells also expand a little, while the third shell suffers contraction. The expansion of the first and second shell consistent with the fact that the ionic radius of Tl1, equal to 1.40 Å, is larger than the ionic radius of Na1 ~0.95 Å!. In summary we find that the structural relaxation around Tl1 impurity in NaI is small, although more complicate than that usually assumed by previous workers. In fact calculations suggest that the relaxation could even go bey the fourth shell.. Let us now turn to CsI:Tl1. The calculation with model (A* ) would give a small expansionDR1 of the first shell if we take as referenceR1. expt(pure crystal), and our calculatio would then be in agreement with that of Berrondoet al.24. However, the ionic radius of Tl1 is lower than that for Cs1; so an expansion ofR1 is not to be expected. By using, in stead, Eq. ~1! we obtained a corrected resultDR1 5 2 0.062 Å, that is, a contraction. Cluster model (C* ), in which only the first shell around Tl1 is allowed to distort, gives a small expansion ofR1 and finally model (D* ) recov- ers again the expected contraction. Beyond the first sh DRi oscillates~DR2 andDR4 are also negative, whileDR3 ,. l. TABLE II. Distortion induced by a Tl1 impurity in NaI and CsI. DistancesRi (i 5 1,2, . . . ) in Å between the Tl 1 and its successive. coordination shells are given, as well as the differencesDRi with respect to the values obtained in calculations for the perfect crystal~also with the cluster model! and percent distortions. The last column gives absorption energies~see text! together with percent deviations from the experimental value.. NaI:Tl1 Cluster R1 R2 R3 R4 DR1 DR2 DR3 DR4 Abs. ~eV!. ~A! 3.738 1 0.198 3.91(2 8.00%) ( 1 5.59%). ~C! 3.274 1 0.061 4.19(2 1.41%) ( 1 1.87%). ~D! 3.273 4.692 5.510 6.612 1 0.039 1 0.075 2 0.054 1 0.043 4.23(2 0.47%) ( 1 1.21%) (1 1.62%) (2 0.97%) (1 0.64%). CsI:Tl1 Cluster DR1 DR2 DR3 DR4 DR5 DR6 Abs. ~eV!. (A* ) 2 0.062 4.17(2 2.34%) ( 2 1.62%). (C* ) 1 0.013 4.21(2 1.40%) ( 1 0.30%). (D* ) 2 0.047 2 0.008 1 0.003 2 0.016 1 0.006 1 0.001 4.26(2 0.23%) ( 2 1.14%) (2 0.15%) (1 0.06%) (2 0.21%) (1 0.09%) (1 0.01%). or ion th s. a io th. cu io w. gy. t. on f. f t f a. se ca cu. t tio re th. n. n tum een ns rom elf-. ana- he but the ob- l ty-. as h- In rs rgies and be-. of ide aw- er- of the or se. ould that del. ice at- ol- an. 11 968 PRB 58AGUADO, AYUELA, LÓ PEZ, AND ALONSO DR5 , andDR6 are positive!, although the values ofDRi are very small, in fact smaller than in NaI:Tl1.. The conclusion from our calculations is that the dist tions around the impurity affect ions in several coordinat shells around the impurity, and that consideration of both atomic and the electronic relaxation of ions in those shell required.. For each active cluster we have also calculated the sorption energy corresponding to the intra-atomic transit from the singlet ground state to the triplet excited state of thallium ion @ 6s2( 1S)→6s16p1( 3P) #. Following the Franck-Condon principle, this absorption has to be cal lated at the frozen ground state geometrical configurat Thus, to obtain the energy of the localized excitation, solve the HFR equations49 for that geometrical configuration of the active cluster, with the Tl1 ion in the excited elec- tronic state 6s16p1( 3P), and evaluate the absorption ener as a difference of effective ionic energies:56. Eabs5 Ee f f@ Tl 1~ 3P!#2 Ee f f@ Tl. 1~ 1S!#. ~2!. To calculate the contribution of an electronic open shell the intra-atomic energy of aLS electronic configuration, the Hartree-Fock-Roothaan formalism requires the coupling c stants of that specificLS term as input. For the description o the open shell ion we have used the coupling constants o 3P term as given in Ref. 57 and the same basis set as Tl1(6s2). The absorption spectra of these doped crystals more structured~there are several absorption bands!; our cal- culated transitions should be identified with the band~A! of the absorption spectrum of NaI:Tl1 ~4.25 eV!,58 and with the first absorption band of CsI:Tl1 ~4.27 eV!.59 Both in NaI:Tl1. and CsI:Tl1, the absorption energies we obtain come clo to experiment as we improve the description of the lo geometry around the impurity, as Table II shows. In parti lar the absorption energies obtained with models~D! and (D* ) are remarkably accurate, and this can be ascribed to accurate representation achieved for the lattice distor around Tl1. Treatment of other absorption bands would quire us to depart from some of the basic assumptions of PI model.. IV. SUMMARY. We have reported a study of the local lattice distortio induced by a Tl1 impurity in NaI:Tl1 and CsI:Tl1 scintilla- .. -. e is. b- n e. - n. e. o. -. he or re. r l -. he n - e. s. tors. To that end, theab initio perturbed ion model has bee used. Large active clusters, embedded in accurate quan environments representing the rest of the crystal, have b studied. The importance of performing parallel calculatio for pure systems in order to suppress systematic errors f calculated local distortions has been stressed. The s embedding performance of the method has been also lyzed with the result that it is necessary to include in t active cluster some shells of ions with frozen positions able to adapt self-consistently their wave functions to displacements of the inner shells. The local distortions tained extend beyond the first shell of neighbors in NaI:T1. Thus, the assumptions frequently employed in impuri cluster calculations, which consider the active space formed by the central impurity plus its first shell of neig boring ions only, should be taken with some care. CsI:Tl1, our results indicate that only the first shell suffe an appreciable displacement. Calculated absorption ene are in excellent agreement with the experimental values, that agreement improves as the description of the cluster comes more realistic.. Thus, the PI model is able to give a realistic description the geometrical distortion around a defect in an alkali-hal crystal. Of course, the advantages come with some dr backs: The simplifying assumptions present in the actual v sion of the PI model make it unsuitable for the study excited states involving interatomic charge transfer from impurity. The method also has difficulties for accounting f the crystal-field splitting of open shell excited states. The drawbacks concerning the treatment of excited states sh not overlook the essential message of this paper, that is, the PI method combined with an embedded cluster mo allows one to obtain accurately the distortion of the latt around impurity centers in ionic crystals. A combined str egy, namely, PI calculations to obtain the distortions, f lowed by a MO calculation on the optimized geometry, c be a desirable option in the future.. ACKNOWLEDGMENTS. Work supported by DGES~PB95-0720-CD2-01! and Junta de Castilla y Leo´ n ~VA63/96!. A. Aguado was sup- ported by Junta de Castilla y Leo´ n. A. Ayuela acknowledges support by the EU TMR program. ci, lids 1G. Blasse and B. C. Grabmaier,Luminescent Materials~Springer- Verlag, Berlin, 1995!.. 2H. Chermette and C. Pedrini, J. Chem. Phys.75, 1869~1981!. 3N. W. Winter, R. M. Pitzer, and D. K. Temple, J. Chem. Phys.86,. 3549 ~1987!. 4A. B. Kunz and J. M. Vail, Phys. Rev. B38, 1058~1988!. 5Z. Barandiara´n and L. Seijo, J. Chem. Phys.89, 5739~1988!. 6V. Luaña and L. Pueyo, Phys. Rev. B39, 11 093~1989!. 7V. Luaña, M. Bermejo, M. Flo´ rez, J. M. Recio, and L. Pueyo, J. Chem. Phys.90, 6409~1989!. 8L. Seijo and Z. Barandiara´n, J. Chem. Phys.94, 8158~1991!. 9J. Andriessen, P. Dorenbos, and C. W. E. van Eijk, Mol. Phys.74, 535 ~1991!.. 10M. S. Islam and R. C. Baetzold, J. Phys. Chem. Solids53, 1105 ~1992!.. 11V. Luaña and M. Flórez, J. Chem. Phys.97, 6544~1992!. 12E. Miyoshi and S. Huzinaga, Phys. Rev. B48, 8583~1993!. 13A. Scacco, S. Fioravanti, M. Missori, U. M. Grassano, A. Lu. M. Palummo, E. Giovenale, and N. Zema, J. Phys. Chem. So 54, 1035~1993!.. 14V. Luaña, M. Flórez, and L. Pueyo, J. Chem. Phys.99, 7970 ~1993!.. ,. a,. an. .. p- n. n. J.. t-. er. ns. J.. nd. -. m. .. .. r. ,. - ns.. PRB 58 11 969LATTICE DISTORTIONS AROUND A Tl1 IMPURITY . . . 15R. Visser, J. Andriessen, P. Dorenbos, and C. W. E. van Eijk Phys.: Condens. Matter5, 5887~1993!.. 16J. Andrés, A. Beltrán, S. Bohm, A. Flores-Riveros, J. A. Igualad V. Luaña, A. Martı́n Penda´s, and G. Monro´ s, J. Phys. Chem.97, 2555 ~1993!.. 17M. Flórez, M. A. Blanco, V. Luan˜a, and L. Pueyo, Phys. Rev. B 49, 69 ~1994!.. 18A. Beltrán, A. Flores-Riveros, J. Andre´s, V. Luaña, and A. Martı´n Penda´s, J. Phys. Chem.98, 7741~1994!.. 19M. Berrondo and J. F. Rivas-Silva, Int. J. Quantum Chem., Qu tum Chem. Symp.29, 253 ~1995!.. 20J. L. Pascual and L. Seijo, J. Chem. Phys.102, 5368~1995!. 21T. J. Gryk and R. H. Bartram, J. Phys. Chem. Solids56, 863. ~1995!. 22R. Llusar, M. Casarrubios, Z. Barandiara´n, and L. Seijo, J. Chem. Phys.105, 5321~1996!. 23L. Seijo and Z. Barandiara´n, Int. J. Quantum Chem.60, 617. ~1996!. 24M. Berrondo, F. Rivas-Silva, and J. B. Czirr,Proceedings of the. International Conference on Inorganic Sintillators and their A plications, SCINT95, edited by P. Dorenbos and C. W. E. va Eyjk ~Delft University Press, Delft, 1996!, p. 144.. 25M. Berrondo and F. Rivas-Silva, Int. J. Quantum Chem.57, 1115 ~1996!.. 26S. Huzinaga, L. Seijo, Z. Barandiara´n, and M. Klobukowski, J. Chem. Phys.86, 2132~1987!.. 27X. Zhang and C. R. A. Catlow, Phys. Rev. B47, 5315~1993!. 28X. Zhang, C. K. Ong, and A. M. Stoneham, J. Phys.: Conde. Matter 6, 5647~1994!. 29M. S. Islam and R. C. Baetzold, J. Mater. Chem.4, 299 ~1994!. 30M. S. Islam and L. J. Winch, Phys. Rev. B52, 10 510~1995!. 31D. C. Sayle, C. R. A. Catlow, M.-A. Perrin, and P. Nortier,. Phys. Chem. Solids56, 799 ~1995!. 32M. J. Akhtar, Z.-D.-N. Akhtar, R. A. Jackson, and C. R. A. Ca. low, J. Am. Chem. Soc.78, 421 ~1995!. 33M. Exner, H. Donnerberg, C. R. A. Catlow, and O. F. Schirm. Phys. Rev. B52, 3930~1995!. 34C. R. A. Catlow, M. S. Islam, and X. Zhang, J. Phys.: Conde. Matter 10, L49 ~1998!. 35C. R. A. Catlow and P. D. Townsend,Point Defects in Materials. ~Academic Press, London, 1998!. 36A. M. Stoneham~unpublished!. J.. -. s.. ,. .. 37J. H. Harding, Rep. Prog. Phys.53, 1403~1990!. 38M. Wilson and P. A. Madden, J. Phys.: Condens. Matter5, 2687. ~1993!. 39M. Wilson, P. A. Madden, N. C. Pyper, and J. H. Harding,. Chem. Phys.104, 8068~1996!. 40J. D. Gale, Philos. Mag. B73, 3 ~1996!. 41J. D. Gale, Faraday Discuss.106, 219 ~1997!. 42V. Luaña and L. Pueyo, Phys. Rev. B41, 3800~1990!. 43V. Luaña, J. M. Recio, and L. Pueyo, Phys. Rev. B42, 1791. ~1990!. 44L. Pueyo, V. Luan˜a, M. Flórez, and E. Francisco, inStructure,. Interactions and Reactivity, edited by S. Fraga~Elsevier, Am- sterdam, 1992!, Vol. B, p. 504.. 45V. Luaña, M. Flórez, E. Francisco, A. Martı´n Penda´s, J. M. Re- cio, M. Bermejo, and L. Pueyo, inCluster Models for Surface and Bulk Phenomena, edited by G. Pacchioni, P. S. Bagus, a F. Parmigiani~Plenum, New York, 1992!, p. 605.. 46V. Luaña, A. Martı́n Penda´s, J. M. Recio, and E. Francisco, Com put. Phys. Commun.77, 107 ~1993!.. 47S. Huzinaga and A. P. Cantu, J. Chem. Phys.55, 5543~1971!. 48S. Huzinaga, D. McWilliams, and A. A. Cantu, Adv. Quantu. Chem.7, 183 ~1973!. 49C. C. J. Roothaan and P. S. Bagus,Methods in Computational. Physics~Academic, New York, 1963!, Vol. 2, p. 47. 50E. Francisco, A. Martı´n Penda´s, and W. H. Adams, J. Chem. Phys.97, 6504~1992!. 51E. Clementi, IBM J. Res. Dev.9, 2 ~1965!. 52S. J. Chakravorty and E. Clementi, Phys. Rev. A39, 2290~1989!. 53W. H. Press and S. A. Teukolsky, Comput. Phys.5, 426 ~1991!. 54E. Clementi and C. Roetti, At. Data Nucl. Data Tables14, 177. ~1974!. 55A. D. McLean and R. S. McLean, At. Data Nucl. Data Tables26,. 197 ~1981!. 56A. Martı́n Penda´s, E. Francisco, V. Luan˜a, and L. Pueyo, J. Phys. Chem.96, 2301~1992!. 57G. L. Malli and J. F. Olive,Vector Coupling Coefficients fo. Atomic Self-Consistent Field Calculations, Laboratory of Mo- lecular Structure and Spectra~University of Chicago, Chicago 1963!, pt. 2, p. 258.. 58P. W. M. Jacobs, J. Phys. Chem. Solids52, 35 ~1991!. 59V. Nagirnyi, A. Stolovich, S. Zazubovich, V. Zepelin, E. Mi. hokova, M. Nikl, G. P. Pazzi, and L. Salvani, J. Phys.: Conde Matter 7, 3637~1995!.